Porous Lanthanide‒Organic Frameworks: Control over Interpenetration, Gas Adsorption, and Catalyst Properties
He, Haiyan; Ma, Huiqing; Sun, Di; Zhang, Liangliang; Wang, Rongming; Sun, Daofeng; Crystal Growth & Design 13 (2013) 3154–; doi:10.1021/cg400531j

data_4510675
_publ_section_title
;
 Porous Lanthanide--Organic Frameworks: Control over Interpenetration, Gas
 Adsorption, and Catalyst Properties
;
_journal_issue                   7
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              3154
_journal_paper_doi               10.1021/cg400531j
_journal_volume                  13
_journal_year                    2013
_chemical_formula_sum            'C48 H30 Er2 N4 O15'
_chemical_formula_weight         1237.28
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                99.7550(10)
_cell_angle_beta                 110.2450(10)
_cell_angle_gamma                107.7930(10)
_cell_formula_units_Z            1
_cell_length_a                   10.0691(6)
_cell_length_b                   10.9491(7)
_cell_length_c                   13.2211(8)
_cell_measurement_temperature    293(2)
_cell_volume                     1238.82(13)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.988
_diffrn_measured_fraction_theta_max 0.988
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0647
_diffrn_reflns_av_sigmaI/netI    0.0762
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            6185
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.05
_exptl_absorpt_coefficient_mu    3.434
_exptl_absorpt_correction_T_max  0.8471
_exptl_absorpt_correction_T_min  0.6269
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_density_diffrn    1.658
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             602
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.360
_refine_diff_density_min         -1.475
_refine_diff_density_rms         0.173
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.003
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     303
_refine_ls_number_reflns         4300
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.003
_refine_ls_R_factor_all          0.0479
_refine_ls_R_factor_gt           0.0366
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0486P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0929
_refine_ls_wR_factor_ref         0.0976
_reflns_number_gt                3665
_reflns_number_total             4300
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg400531j_si_002.cif
_cod_data_source_block           p3
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4510675